### A dispersive homogenization model for composites and its RVE existence

Liu, Y.; van der Meer, F. P.; Sluys, L. J. DOI

10.1007/s00466-019-01753-9 Publication date

2019

Document Version Final published version Published in

Computational Mechanics

Citation (APA)

Liu, Y., van der Meer, F. P., & Sluys, L. J. (2019). A dispersive homogenization model for composites and its RVE existence. Computational Mechanics, 65 (2020)(1), 79-98. https://doi.org/10.1007/s00466-019-01753-9

Important note

To cite this publication, please use the final published version (if applicable). Please check the document version above.

Copyright

Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons. Takedown policy

Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.

https://doi.org/10.1007/s00466-019-01753-9
**O R I G I N A L P A P E R**

**A dispersive homogenization model for composites and its RVE**

**existence**

**Y. Liu1· F. P. van der Meer1· L. J. Sluys1**

Received: 4 February 2019 / Accepted: 12 July 2019 / Published online: 29 July 2019 © The Author(s) 2019

**Abstract**

An asymptotic homogenization model considering wave dispersion in composites is investigated. In this approach, the effect of the microstructure through heterogeneity-induced wave dispersion is characterised by an acceleration gradient term scaled by a “dispersion tensor”. This dispersion tensor is computed within a statistically equivalent representative volume element (RVE). One-dimensional and two-dimensional elastic wave propagation problems are studied. It is found that the dispersive multiscale model shows a considerable improvement over the non-dispersive model in capturing the dynamic response of heterogeneous materials. To test the existence of an RVE for a realistic microstructure for unidirectional fiber-reinforced composites, a statistics study is performed to calculate the homogenized properties with increasing microstructure size. It is found that the convergence of the dispersion tensor is sensitive to the spatial distribution pattern. A calibration study on a composite microstructure with realistic spatial distribution shows that convergence is found although only with a relatively large micromodel.

**Keywords Composites**· Wave dispersion · Homogenization · RVE · Spatial distribution

**1 Introduction**

The heterogeneity of the microstructure of composite mate-rials causes dispersion in wave propagation associated with dynamic loading. This dispersion phenomenon, also referred to as micro-inertia, is a result of local motion of the microstructure driven by multiple wave reflections and trans-missions occurring at the interfaces between the constituents. Correct evaluation or tuning of the dispersion properties of composites can be important for engineering applications, for instance impact-resistant components or devices where composites are subject to high-rate loading [1–5] or meta-materials with microstructures designed to show particular effective behavior [6–8].

**Electronic supplementary material** The online version of this article
(https://doi.org/10.1007/s00466-019-01753-9) contains

supplementary material, which is available to authorized users.

### B

Y. Liu1 _{Faculty of Civil Engineering and Geosciences, Delft}
University of Technology, P.O. Box 5048, 2600 GA Delft,
The Netherlands

Computational modelling of composites subjected to stress-wave loading typically involves three length scales, i.e. the size of the macroscopic structure, the characteristic stress wave length and the length scale of the microstructure (in fiber-reinforced composites related to the fiber diameter) [8,9]. The macroscopic length scale can be much larger than the microstructural length scale. In the case where the stress wave length is also much larger than the typical microstruc-tural size, there is no significant transient effect within the microstructure and micro-inertia is negligible [8]. Therefore, the overall dynamic response can be solely described by averaging density and moduli. However, for a stress wave which is only few times larger than the microstructural length scale, the dispersion becomes evident and averaging proper-ties are not sufficient to describe the dynamic response [8]. In order to account for the dispersion phenomenon, mul-tiple models have been introduced. One type of model is the gradient elasticity model with high-order spatial deriva-tives of strains, stresses and/or accelerations as reviewed by Askes and Aifantis [10]. However, identification of the length-scale parameters of this method, especially in a multi-dimensional context, is not totally clear. Besides, Willis’ elastodynamics homogenization model derives an effective constitutive relation which introduces non-classical coupling

between effective stress and effective velocity and coupling between effective momentum and effective strain [11–14]. Recent development of generalized homogenization models enrich the macroscale displacement with additional general-ized degrees of freedom of Bloch modes following the lines of Willis’ model, see Sridhar et al. [15]. These methods are suitable for linear elastic (layered) periodic materials while an extension to materials with random microstructure is not always straightforward.

An alternative type of method which provides a more flexible framework (e.g. consideration of complex random microstructure or material nonlinearity) is representative vol-ume element (RVE) based multiscale approaches. Initiated by Hill [16], the RVE can be defined as a characteristic sam-ple of heterogeneous material that should be large enough to contain sufficient composite micro-heterogeneities in order to be representative, however it should be much smaller than the macroscopic structure size. Several definitions of an RVE are introduced in literature, as reviewed by Gitman et al. [17]. Generally, a micromodel can be considered represen-tative if further increase of its size of RVE does not lead to changes in the homogenized properties. Typically, statistics studies using numerical computations are used to evaluate the homogenized physical properties (e.g. elastic properties, thermo-conductivity) or effective response (e.g. the effective stress) of a range of micromodels with increasing size, for instance in [17–24]. It should be noted that the size of an RVE depends on the specific investigated morphological (e.g. vol-ume fraction) or physical properties (e.g. thermal or elastic) [18,20].

Multiscale methods assume multiple (at least two) spa-tial and (or) temporal scales [25,26]. In multiscale models finer-scale problems are considered in a (statistically equiva-lent) representative volume element (RVE) and information of the finer-scale is hierarchically passed into a coarser scale by bridging laws. Based on a multiscale virtual power principle [25] as a notion of a generalized Hill-Mandel lemma, Pham et al. [8] and Roca et al. [27] developed computational homogenization schemes in which the tran-sient dynamics equations are resolved at macroscopic and microscopic scale. Asymptotic homogenization with higher-order (or first-higher-order) expansions was proposed in [28–30] to capture wave dispersion and attenuation within viscoelastic composites. Fish et al. [31] introduced a general purpose asymptotic homogenization scheme in which the micro-inertia is resolved by introducing a eigenstrain term and is valid for nonlinear heterogeneous material. This method was further investigated by Karamnejad and Sluys [32] for impact-induced crack propagation within a heterogeneous medium. The aforementioned methods have shown certain capabilities in capturing wave dispersion for strictly periodic heterogeneous structures with simple microstructures where the RVE can be clearly defined as a unit cell. However, in a

realistic composite material, the microstructure has a random nature. Therefore, the question of RVE existence needs to be answered before multiscale methods can be employed.

In this paper, a dispersive multiscale model based on asymptotic homogenization is reviewed and the existence of an RVE for this method for unidirectional fiber-reinforced composites is investigated. This paper is organized as fol-lows: in Sect.2, the dispersive model based on asymptotic homogenization technique is introduced. The accuracy of this numerical method for 1D and 2D elastic wave propagation is demonstrated in Sect. 3. In Sect. 4, a statistics study is performed to investigate if an RVE exists for this homog-enization approach for realistic fiber reinforce composite microstructures. In Sect.5, a batch of calibrated numerical samples based on experimentally determined spatial distri-bution pattern is tested for the convergence of homogenized properties.

**2 Dispersive homogenization model**

In this section, the asymptotic homogenization model origi-nated from Fish et al. [31] and later explored by Karamnejad and Sluys [32] is described. This method allows for a decou-pling of the equation of motion into a two-scale formulation. The effect of microscopic dispersion is quantified by a so-called “dispersion tensor”, which is related to the acceleration influence function of the microstructure. The acceleration influence functions for microstructures with one and multi-ple inclusions are demonstrated as exammulti-ples.

**2.1 Two-scale formulation**

Considering a composite structure that is in dynamic equi-librium with prescribed displacements and stress boundary conditions and given the initial conditions for displacement and velocity (see Fig. 1a), the linear momentum equation reads

*∂σi jζ*

*∂xζ _{j}*

*= ρ*

*ζ _{¨u}ζ*

*i,* in*ζ* (1)

with boundary conditions

*uζ _{i}(x, t) = uζ_{i}(x, t) on ∂uζ* (2)

*σi jζ*

**(x, t)n**ζj**(x) = t**ζi**(x, t) on ∂***tζ*

(3)
at the boundary surface *∂ζ* *= ∂uζ* *∪ ∂tζ* and initial
displacement and velocity conditions

*u _{i}ζ(x, 0) = u*0

*(4)*

_{i}**(x)***˙uiζ (x, 0) = v*

0

**Fig. 1 Problem statement. a**

**Original composite problem; b**
equivalent two-scale problem

statement _{Ω}ζ
**(a)** **(b)**
*x*ζ_{1}
*x*ζ_{2}
*n*ζ
*x*1
*x*2
Ω
*t*
*t*ζ
*n*
×1
ζ
*y*1
*y*2
Θ
*yi= xi*/ζ

where* σζ*,

*ρζ*

**, u**ζ*are stress, density, displacement and surface outward normal, respectively. The superscript*

**and n**ζ*ζ denotes that quantities are defined within the composite*domain. For simplicity, a linear elastic material law is con-sidered herein, namely

*σi jζ (x, t) = S*

*ζ*

*i j kl*

**(x)ε***ζ*

*kl (x, t)* (6)

where**ε**ζ* is strain and Sζ* is the elastic stiffness tensor which
is for two-phase (i.e. inclusion and matrix) composites a
piece-wise constant function of spatial coordinates.
Exten-sion to nonlinear material behavior can be done by using
the instantaneous stiffness tensor as elaborated in Fish et
al. [31]. Perfect bonding between inclusion and matrix is
considered here while decohesion can be possibly included
through the eigendeformation concept [33] or a cohesive
crack formulation [34]. A relevant study on dispersive
mul-tiscale formulation with consideration of material damage is
introduced by Karamnejad and Sluys [32].

**2.1.1 Asymptotic expansions**

In the asymptotic expansion approach, two spatial coordinate
* systems are introduced, macro-scale coordinates x defined in*
the macroscopic homogeneous domain

*and micro-scale*

**coordinates y in an RVE domain***with heterogeneous*microstructures, see Fig.1

**b. The y coordinate is related to**

**the x coordinate by y****= x/ζ with 0 < ζ 1. Any**

**physi-cal field variable, for example, the displacement field u, is a**

**function of spatial coordinate x, y and also the physical time***domain*

**t . These physical fields are assumed to be y-periodic in RVE**

**, namely f (x, y) = f (x, y+kl**R) in which vector**l**R*= [l*1*, l*2]*T* represents the basic period of the

*microstruc-ture (in 2D), l*1*and l*2are the lengths of RVE along the two

* directions and k is a 2*× 2 diagonal matrix with integer
com-ponents. The choice for periodic boundary conditions for the

microscopic field is motivated by superior convergence
prop-erties that have been demonstrated by Kanit et al. [18] and
Fish [35] among others. Following Fish et al. [31], we can
represent this function by an asymptotic expansion around a
**point x in powers of**ζ , namely,

* uζ(x, t) = u(0)(x, t) + ζ u(1)(x, y, t) + O(ζ*2

*)*(7) in which the first term on the right hand side represents a macro-scale component while the second term represents a micro-scale component. By applying the two-scale spatial derivative rule

*∂(·)ζ*

*∂xiζ*

= *∂(·) _{∂x}_{i}*+1

*ζ∂(·)∂ yi*, the strain can be expressed

as
*εζi j (x, t) ≡ uζ_{(i,x}ζ*

*j)*

**(x, t)***= εm*

*i j*

**(x, y, t) + O(ζ )***= u(0) _{(i,x}_{j}_{)}(x, t) + u(1)_{(i,y}_{j}_{)}(x, y, t) + O(ζ )* (8)
where

*εm*is the micro-scale strain and

_{i j}*(·)*=

_{(i,x}j)1
2
*∂(·)i*
*∂xj*
+*∂(·)j*
*∂xi*

means the symmetric gradient of a function with
**respect to coordinate x. The stress is expanded as**

*σi jζ (x, t) = σ*

*m*

*i j (x, y, t) + O(ζ )*

*= σi j(0) (x, t) + σi j(1)(x, y, t) + O(ζ )* (9)

where*σ _{i j}m*is the micro-scale stress and the micro-scale
per-turbation stress

*σ*satisfies

_{i j}(1)*σi j(1) (x, y, t) = 0* (10)

where*(·) =* * _{||}*1

*within the domain*

_{}(·)d is the volumetric average of (·)*.*

The inertia is given as the following expansion
*ρζ _{¨u}ζ*

*i*

**(x, y, t) = ρ**(0)¨u*(0)*

*i*

**(x, t) + ζρ**(1)¨u*(1)*

*i*

*2*

**(x, y, t) + O(ζ***)*

*= ρ(0)*

_{¨u}(0)*i*

**(x, t) + ζρ**(0)hsti**(x, y, t)¨ε**(0)st*2*

**(x, t) + O(ζ***)*(11)

*where hst*

_{i}*function which satisfies*

**(x, y, t) is the so-called acceleration influence***ρ(1)¨u(1)*

_{i}*= ρ(0)hst*

_{i}*¨εst(0)and hsti*

**(x, y,***t) is a y-periodic function satisfying the normalization *
con-dition

*hst*

*i* * (x, y, t) = 0* (12)

**2.1.2 Weak form**

The weak form of Eq. (1) reads
*ζω*
*ζ*
*i, jσ*
*ζ*
*i jdζ*+
*ζω*
*ζ*
*iρζ¨u*
*ζ*
*idζ* =
*∂tζω*
*ζ*
*it*
*ζ*
*idζ*
(13)
in which the test function *ω _{i}ζ*

*∈ Wζ*

*= {ωζ*

_{i}*∈ C*0

*(ζ),*

*ωiζ*

*= 0 on ∂uζ*}. Integration of the two-scale functions

over the composite domain and its boundary is carried out as

*ζ(·)d*
*ζ*_{= lim}
*ζ→0*
·*d and*
*∂ζ(·)d*
*ζ*_{=}
*∂(·)d*
(14)
The test function is expanded as

*ωiζ (x, t) = ωi(0)(x, t) + ζ ω(1)i*

*2*

**(x, y, t) + O(ζ**

_{)}*= ωi(0)*

**(x, t) + ζ h***kl*

*i*

*2*

**(x, y, t)ω**(0)_{(k,x}l)**(x, t) + O(ζ***(15) where the relation*

_{)}*ω(1)*

_{i}

**(x, y, t) = h**kl_{i}

**(x, y, t)ω**_{(k,x}(0)*l) (x, t) is*

introduced.

By applying the two-scale integration scheme Eq. (14) to Eq. (13) and using Eqs. (9), (10), (11), (12) and (15) and neglecting higher-order terms, it can be found that

*ω*
*(0)*
*(i,xj)*
*σi j(0)+ ζ*
2
*Di j st¨εst(0)*
*d*
+
*ω*
*(0)*
*i* *ρ(0)¨u(0)i* *d*
+
*ω*
*(1)*
*(i,yj)σ*
*m*
*i j**d =*
*∂t* *ω*
*(0)*
*i* *tid* (16)
where*ω(0) _{i}*

*∈ W(0)*

*= {ω(0)*

_{i}*∈ C*0

_{(), ω}(0)*i*

*= 0 on ∂u*} and

*ω*

_{i}(1)*∈ W= {ω*0

_{i}(1)∈ C*(), ω*

_{i}(1)*= 0 on*

_{}= 0, ω_{i}(1)*∂u*is introduced as

**} and the dispersion tensor D**M*D*

_{i j st}M*= ζ*2

*Di j st*(17)

**(x, t) = ρ**(0) hi jp**( y, t)h**stp**( y, t)**where*(·)M* denotes the macro-scale quantity. Therefore, the
weak form for the two scales can be derived as

*ω*
*(0)*
*(i,xj)*
*σi j(0)+ ζ*
2
*Di j st¨ε(0)st*
*d +*
*ω*
*(0)*
*i* *ρ(0)¨ui(0)d*
=
*∂t* *ω*
*(0)*
*i* *tid (macro-scale)* (18)
1
*||*
*ω*
*(1)*
*(i,yj)σ*
*m*
*i jd = 0 (micro-scale)* (19)

The solution of these weak forms is found with separate
finite element schemes for the two scales. Details about the
*extraction of the macro-scale stiffness S _{i j kl}M* are explained in
“Appendix A” and the solution of the micro-scale problem is
illustrated in the next section.

**2.1.3 Micro-scale problem**

It can be observed from Eq. (19) that the micro-scale problem
is treated as a “quasi-dynamic” formulation following Fish et
al. [31*]. Considering that S _{i j kl}ζ*

**(x) = S**_{i j kl}m*the first order remnants in Eqs. (8) and (9), the constitutive relation Eq. (6) can be rewritten as*

**( y) and leaving out***σm*
*i j (x, y, t) = S*

*m*

*i j kl*

**( y)ε***m*

*kl*(20)

**(x, y, t)**The micro-scale strain*εm _{kl}(x, y, t) is divided into two parts:*

*one is caused by the macro-scale strain u(0)*

_{(i,x}*j) (x, t); the other*

one is driven by the macro-scale acceleration gradient. The micro-scale strain, from Eq. (8), is expressed as

*εm*
*kl (x, y, t) = u(0)_{(k,x}l)(x, t) + u*

*(1)*

*(k,yl)*

**(x, y, t)***= u(0)*

_{(k,x}_{l}_{)}**(x, t) + H**st*(k,yl)*

**(x, y, t)u***(0)*

*(s,xt)*

**(x, t)**macro-scale strain related terms

+**ρ( y)***ρ(0)* *fkl(0) (x, t) + h*

*st*

*(k,yl)*

**(x, y, t) f***(0)*

*st*

**(x, t)**macro-scale acceleration gradient related terms

(21)
*where H _{k}st* is a displacement influence function satisfying

**y-periodicity and***H*

_{k}st

_{}*= 0, and f*macro-scopic quantity proportional to the macro-scale acceleration

_{kl}(0)**(x, t) is a***gradient so that f*≡ 0 in the absence of macro-scale accel-eration gradient. It is to be noted that in Eq. (21) the first of the macro-scale strain related terms corresponds to a uni-form strain on the microstructure while the second term is a fluctuation contribution to keep the microstructure to be in self-balanced state. Similarly, the first term of macro-scale acceleration gradient related parts in Eq. (21) represents a uniform acceleration gradient over the microstructure while

_{kl}(0)the second terms refers to a fluctuation contribution to keep the microstructure in equilibrium under the excitation of a macroscopic acceleration gradient.

Substituting Eqs. (20) and (21) into Eq. (19) leads to

*ω*
*(1)*
*(i,yj)*
*Si j klm* **( y)***Iklst+ H_{(k, y}st*

*l)*

**( y, t)***u(0)*

_{(s,x}_{t}_{)}**(x, t)***d*+

*ω*

*(1)*

*(i,yj)*

*Si j klm*

**( y)**

_{ρ( y)}*ρ(0)Iklst+ hst*

_{(k, y}_{l}_{)}**( y, t)***fst(0)*

**(x, t)***d = 0*(22)

*where Iklst*

*= δksδlt*and

*δks*is the Kronecker delta tensor.

*Considering the arbitrariness of u(0) _{(s,x}*

*t)and f*
*(0)*

*st* , Eq. (22) can

be split into two separate equations
*ω*
*(1)*
*(i,yj)*
*Si j klm* **( y)***Iklst+ H_{(k, y}st*

_{l}_{)}**( y, t)***d = 0*(23) and

*ω*

*(1)*

*(i,yj)*

*S*

_{i j kl}m

**( y)**

**ρ( y)***ρ(0)*

*Iklst+ hst*

_{(k, y}_{l}_{)}**( y, t)***d = 0*(24) Of these, the second one is solved for the acceleration

*influ-ence function hst*with finite elements over the micro-scale domain. Details about the solution procedures of Eq. (24) are given in “Appendix B”. By use of Eq. (17

_{k}*), hst*gives the dis-persion tensor which is used in the macro-scale weak form, i.e. Eq. (18).

_{k}**2.2 Acceleration influence functions**

The effect of inertia in the micro-scale is considered by
an eigenstrain [36] and therefore only the solution of a
typical quasi-static balance problem is needed. As it is
pointed out in Fish et al. [31], it is possible to get a closed
form solution of the micro-scale balance Eq. (19) in the
case of a 1D composite bar with two different phases of
*material with elastic material constants of E*1,*ρ*1 *and E*2,
*ρ*2.

For a microstructure with one circular inclusion, the six
acceleration influence functions are plotted in figure2. The
elastic modulus, Poisson’s ratio, mass density of the inclusion
*and matrix are Ei* *= 200 GPa, νi* *= 0.2, ρi* *= 10,000 kg/m*3

*and Em* *= 2 GPa, νm* *= 0.2, ρm* = 4000 kg/m3. The volume

fraction of the inclusion is 60% and its diameter is 5µm.
From Eq. (21), it is known that the acceleration influence
*functions hmn _{k}* can be interpreted as the first-order
microstruc-tural correction to the eigendeformation field as triggered
by the macro-scale acceleration gradient. For instance, the

*negative gradient of h*11

_{1}

*along y*1-direction in the domain

occupied by the stiff inclusion implies that the true accel-eration induced strain in the inclusion is smaller than that

in the matrix domain. For a microstructure with 25× 25
randomly positioned inclusions while keeping the other
*prop-erties unchanged, the influence function h*11_{k}*(k = 1, 2) is*
plotted in Fig. 3. Some observations can be made: (1) the
*gradient h*11* _{(1,y1)}*in the inclusions phase is still negative and
has similar magnitude among all the inclusions, and (2) both

*h*11

_{1}

*and h*11

_{2}show regions where peaks are higher and regions where peaks are lower as a consequence of the mesostruc-ture.

**2.3 Properties of dispersion tensor**

The magnitude of the dispersion tensor depends on
sev-eral characteristics of the microstructure. (i) The contrast
of material properties between the constituents. In terms
of a one-dimensional two-phase composite bar, if the wave
impedance is the same for the two phases, the dispersion
ten-sor is null [31]. This is consistent with the fact that when the
wave impedance is the same, wave dispersion due to
mate-rial heterogeneity is not present. To investigate the influence
of material contrast on the dispersion tensor, the dispersion
tensor is computed for a single microstructure with 15× 15
fibers and a fiber volume fraction of 60%. The Young’s
mod-ulus and density of the inclusion are varied proportionally
*as Ei* *= cEm* and *ρi* *= cρm* *for c* *∈ [2, 4, 9, 16, 30],*

respectively, with the Poisson’s ratio unchanged. The six
*independent components of the dispersion tensor D _{i j kl}M* ,
nor-malized with respect to the values of the sample with the

*lowest property contrast, D*

_{i j kl}M*(c = 2), for the five cases*are shown in Fig. 4a. It can be seen that the magnitude of all six components are increasing with larger properties contrast, which means that the expected dispersion effect should be larger for a higher contrast composite. (ii) The diameter of inclusions. Similarly, the dispersion tensor is computed for five cases with the same material properties and microstructure with 15× 15 inclusions but with

*differ-ent inclusion diameter, di*

*∈ [0.005, 0.025, 0.1, 0.25, 0.5]*

*mm. The variation of D*_{1111}*M* *as function of di* is plotted in

Fig.4b along with a quadratic fit. It can be observed that the
*relation between D*_{1111}*M* *and di* can be described very well as

a quadratic relation and the same was found for the other
components of the dispersion tensor. This quadratic
rela-tion can also be found in the closed-form solurela-tion of the
dispersion tensor for a one-dimensional two-phase
compos-ite bar given in [31]. This means that for larger inclusions,
the influence of dispersion is larger. To ensure a
*mesh-independent solution of D*_{1111}*M* , five different mesh sizes
*of the case with the fiber diameter di* *= 0.25 mm are*

solved, with the number of elements ranging from 22,624
to 288,800. It is shown in Fig.4c that after the mesh size
has reached the medium size, the dispersion tensor
*compo-nent D*_{1111}*M* has reached converged values. Therefore, this

geometry
*y*1(
*y*2(
*h*11
1 (
*y*1(
*y*2(
*h*11
2 (
*y*1(
*y*2(
*h*22
1 (
*y*1(
*y*2(
*h*22
2 (μm)
*y*1(
*y*2(
*h*12
1 (
*y*1(μm)
*y*2(μm)
*h*12
2 (μm)
μm)
μm)
μm)
μm)
μm)
μm)
μm)
μm)
μm)
μm)
μm) μm)
μm) _{μ}_{m)}

* Fig. 2 Acceleration influence function hmn_{k}* for a one inclusion microstructure (the enclosed subfigure shows the studied microstructure)

mesh size is adopted for the study described in Sects. 4

and5.

**3 Comparison with direct numerical**

**simulation**

In this section, elastic wave propagation in a periodic com-posite medium is simulated to investigate the performance of the introduced dispersive homogenization model in compar-ison with direct numerical simulation (DNS). Two cases are

considered, one with a one-dimensional microstructure and one with a two-dimensional microstructure.

**3.1 1D elastic wave propagation**

Elastic wave propagation in a periodic two-phase composite
bar is studied similar to Karamnejad and Sluys [32].
Geom-etry and properties are such that wave propagation is purely
one-dimensional. The material properties of the two phases
*are E*1 *= 200 GPa, ρ*1*= 10,000 kg/m*3,*ν*1 *= 0 and E*2 =

* con-Fig. 3 Influence function h*11
1

*and h*11

_{2}for a 25× 25 inclusions microstructure (the enclosed subfigure shows the studied microstructure)

*h*11 1 (

*y*2(μm)

*y*1(

*h*11 2 (

*y*2(

*y*1( geometry μm) μm) μm) μm) μm)

*trast between the two phases is E*1*ρ*1*/E*2*ρ*2= 250. The left

end of the bar is fixed. Two types of loading are considered.
Firstly, a incoming harmonic wave is imposed on the right
*end of the bar so that the horizontal displacement u(t) on the*
*right edge satisfies u(t) = A*0sin*(2π f t)H( _{2 f}*1

*−t) in which*

*A*0

*= 0.025 mm represents the magnitude, f = 50,000 Hz is*

*the wave frequency and H(·) is the Heaviside step function.*
The bar consists of 100 repeating unit cells for a total length
of 500 mm as shown in Fig.5. Four numerical models are
considered: two single-scale models, namely the fine
hetero-geneous model (DNS) and the fine model with homogenized
properties, and two multiscale models, namely the coarse
non-dispersive model and the coarse dispersive model. The
two fine models consist of 4500 quadrilateral elements. For
the one with homogenized properties, the elastic modulus and
density of the two phases are prescribed to be the
*homoge-nized values, i.e. EM* *= 4.926 GPa and ρM* = 7600 kg/m3,
respectively. This model therefore neglects wave

reflec-tion and transmission at material interfaces. By contrast,
the heterogeneous DNS model considers the
heterogene-ity of the composite bar and is therefore considered as the
reference exact solution of this problem. The two coarse
multiscale models use 500 quadrilateral elements with one
Gauss-integration point corresponding to a unit cell domain.
Homogenized elastic properties are used and the analysis is
performed with and without dispersion tensor. The main
*dis-persion tensor component D*_{1111}*M* for this simple
microstruc-ture can be obtained by a closed-form solution following Fish
et al. [31]. The dispersion tensor is evaluated numerically as

* DM* =
⎡
⎣0

*.0095 0*0 0 00 0 0 0

*.0095*⎤ ⎦ MPa · ms2 (25)

It is shown in Karamnejad and Sluys [32] and Fish et al.
[31*] that the ratio between macroscopic wave length lM* and
*the unit cell size lmdetermines the extent of dispersion. If lM*

**Fig. 4 Properties of dispersion**

**tensor. a Normalized dispersion**
**tensor components; b dispersion**
*tensor component DM*

1111versus
**diameter of inclusion; c mesh**
*density influence of D*_{1111}*M* (the
dashed line shows the converged
mesh size)
101 _{10}2 _{10}3
100
101
102
103
*(Ei*ρ*i)/ (Em*ρ*m*)
*D*
*M* *ijk*
*l*
/
*D*
*M* *ijk*
*l*
*(c*
=2
)
*i jkl = 1111*
2222
1212
1122
2212
1112
geometry
**(a)**
0 0.1 0.2 0.3 0.4 0.5 0.6
0
1
2
*di*(mm)
*D*
*M* 1111
(MP
a·ms
2) geometry
·10−4
*DM*
1111*= 0.00081d*
2
*i*
**(b)**
0 1000000 200000 300000
0.5
0.6
Number of elements
*D*
*M* 1111
(MP
a·ms
2) _{geometry}
·10−4

Selected mesh size

**(c)**

*is more than five times larger than lm*, the dispersive effect
can be neglected. The dispersive model shows considerably
better accuracy than the non-dispersive model within the first
pass frequency band1. In this case, the wave length is
*calcu-lated by lM* =*EM _{(ρ}M_{)}*

_{−1}

_{/ f = 16.1 mm, while the unit}*cell size lm* *= 5 mm. Therefore, the ratio lm/lM* *= 0.3106*
in this case, which corresponds to a shorter wave length than
Karamanejad and Sluys [32]. The displacement field along
the bar is plotted for four typical time instants in Fig.6. It
can be seen in the DNS reference solution that the input
sinu-soidal pulse is not maintained during the propagation and
there exists significant amplitude decay. The resultant
dis-placement field shows sharp kinks representing high velocity
gradients. This flutter characteristic is mainly due to the
high wave impedance contrast between the two phases of
the structure, which causes wave reflection. The result of
the fine homogenized model shows a well maintained profile
although with a small amount of leading oscillation related
to the discretization. A comparison between the DNS model
and fine homogenized model shows that dispersion is indeed

1_{According to Andrianov et al. [}_{37}_{], a periodic elastic composite}
behaves like a discrete wave filter. A discrete pass frequency band and
stop frequency band structure is formed. Whenever the wave frequency
is within the stop frequency band, its magnitude is exponentially
atten-uated such that the wave is not able to propagate. Only when the wave
frequency is within the pass frequency bands, propagation is admissible.

significant for the studied wave length. The solution from the coarse non-dispersive model shows very strong oscillations due to numerical dispersion effects caused by a coarse mesh and the match with the DNS model solution is poor. The coarse dispersive model shows a relatively smooth response. This is because for the dispersive model there is no phys-ical interface in the macro-scale model, so the wave can not “feel” the interface. Nevertheless, there exists reason-ably good agreement between the dispersive solution and the DNS model solution before wave reflection at the left edge (a-c) and after reflection (d) although the dispersive model predicts a stronger decay of magnitude for the oscillation at the rear of the wave. A higher order homogenization scheme could result in a higher accuracy but with more computational costs, see for instance [38].

Secondly, loading which mimics an impact-induced
load-ing pulse is considered, to demonstrate the capability of the
introduced dispersive numerical model for impact problems.
The problem setting is the same as described in Fig.5except
that the horizontal displacement on the right edge is
pre-scribed as
*u(t) =*
⎧
⎪
⎪
⎪
⎨
⎪
⎪
⎪
⎩
*V*
*2Tt*2*,* *t≤ T*
*V T*
2 *+ A · (t − T ),* *T* *< t ≤ 2T*
*2V T* −* _{2T}A(3T − t)*2

*, 2T < t ≤ 3T*

*2V T,*

*t> 3T*(26)

**Fig. 5 Harmonic wave**

propagating in a periodic bar consisted of 100 unit cells. The microstructure of the unit cell is demonstrated 500 mm incoming wave unit cell 1 mm 3 mm 1 mm 1m m Phase 1 Phase 2 0 100 200 300 400 500 -0.01 -0.005 0 0.005 0.01 0.015 0.02 0.025 0.03 Fine heterogeneous (DNS) Fine homogenized Coarse non-dispersive Coarse dispersive (proposed)

x-coordinate (mm)
Displacement
(mm)
**(a)**t = 0.1 ms
0 100 200 300 400 500
-0.01
-0.005
0
0.005
0.01
0.015
0.02
0.025
0.03
x-coordinate (mm)
Displacement
(mm)
**(b)**t = 0.3 ms
0 100 200 300 400 500
-0.01
-0.005
0
0.005
0.01
0.015
0.02
0.025
0.03
x-coordinate (mm)
Displacement
(mm)
**(c)**t = 0.5 ms
0 100 200 300 400 500
-0.03
-0.025
-0.02
-0.015
-0.01
-0.005
0
0.005
0.01
x-coordinate (mm)
Displacement
(mm)
**(d)**t = 0.9 ms

**Fig. 6 Plots of displacement field at different time for DNS-heterogeneous, DNS-homogeneous, dispersive multiscale and non-dispersive multiscale**

model

*in which V and T are constants. This corresponds to a *
trape-zoidal velocity pulse shown in Fig.7. Two load periods are
*considered for this type of loading: (1) T* *= 0.01 ms and*
*(2) T* *= 0.001 ms with the same V = 5.0 m/s. The *
dis-placement field for two typical time instants along the bar
for four models, i.e. the fine heterogeneous model (DNS),
the fine homogenized model, the coarse non-dispersive
mul-tiscale model and the coarse dispersive mulmul-tiscale model, is

*t*
*˙u(t)*

*V*

*T* *2T* *3T*

**Fig. 7 Loading pulse of velocity***˙u(t) applied at the right edge of the*

0 100 200 300 400 500 -0.02 0 0.02 0.04 0.06 0.08 0.1 0.12 Fine heterogeneous (DNS) Fine homogenized Coarse non-dispersive Coarse dispersive (proposed)

x-coordinate (mm)
Displacement
(mm)
**(a)***t = 0.23 ms*
0 100 200 300 400 500
-0.02
0
0.02
0.04
0.06
0.08
0.1
0.12
x-coordinate (mm)
Displacement
(mm)
**(b)***t = 0.4 ms*

**Fig. 8 Plots of displacement field at different time instants for loading pulse with T**= 0.01 ms

0 100 200 300 400 500 -2 0 2 4 6 8 10 12 14 10 -3 x-coordinate (mm) Displacement (mm) Fine heterogeneous (DNS) Fine homogenized Coarse non-dispersive Coarse dispersive (proposed)

**(a)***t = 0.09 ms*
0 100 200 300 400 500
-2
0
2
4
6
8
10
12
14 10
-3
x-coordinate (mm)
Displacement
(mm)
**(b)***t = 0.2 ms*

**Fig. 9 Plots of displacement field at different time instants for loading pulse with T**= 0.001 ms

plotted in Figs.8and9 for the two loading periods. It can be found that dispersion is significant in both cases as the DNS solution is different from the fine homogenized model solution. The second case with shorter time duration shows more evident dispersion. For both cases, the coarse dispersive model shows a better agreement with the DNS model than the non-dispersive model. From the examples of a harmonic loading and a trapezoidal loading, it is concluded that the dis-persive multiscale model offers considerable improvements over the non-dispersive model for 1D elastic wave propaga-tion problems. The dispersive multiscale model allows for

capturing dispersion with a discretization at macroscale that is coarser than the microstructural resolution.

**3.2 Two-dimensional wave propagation**

Next, elastic wave propagation in a material with a two dimensional microstructure subjected to an incoming sinu-soidal wave is considered. The geometry consists of 100 repeating microstructures with a total length of 57.04 mm. There are two phases of materials, circular inclusions with a diameter of 0.5 mm and a surrounding matrix. The top

**Fig. 10 The DNS model mesh**

(501,170 linear triangular elements)

unit cell

100 repeating cells
**Fig. 11 The multiscale model**

(500 linear quadrilateral elements)

edge and bottom edge of the structure are fixed in vertical
direction, which together with plane-strain conditions
mim-ics the state for materials in the middle region along the
thickness direction for a plate impact test [39]. The horizontal
*displacement u*1of the incoming wave at the right edge

*sat-isfies u*1*= A*0sin*(2π f t)H( _{2 f}*1

*− t) with A*0

*= 0.025 mm*

*and f* = 400 KHz with constrained vertical displacement
*u*2 = 0. The elastic properties of inclusion and matrix are

*the Young’s modulus Ei* *= 200 GPa, Em* = 2 GPa, density

*ρi* *= 10,000 kg/m*3, *ρm* = 4000 kg/m3, and the

Pois-son’s ratio *νi* *= 0.2, νm* *= 0.33. The volume fraction*

*of inclusions Vi* is 60%. Similar to Sect.3.1, four

numer-ical models are considered: the fine heterogeneous model (DNS), the fine model with homogenized properties, the coarse non-dispersive multiscale model and the coarse dis-persive multiscale model. The fine models are discretized with 501,170 linear triangular elements (see Fig.10). For the homogenized one, the material properties of the com-plete domain are prescribed to be the homogenized values of each phase. By contrast, the DNS model keeps the different properties of each phase and therefore the dispersion caused by material heterogeneity is naturally included. The coarse models are discretized with 500 linear quadrilateral elements at the macro-scale while each Gauss integration point corre-sponding to a micro-scale problem solved within a unit cell domain as shown in Fig.11. The coarse non-dispersive model neglects the contribution of dispersion at the macro-scale while the dispersive model adds the dispersion tensor contri-bution to capture the dispersion effect. The RVE for this struc-ture is clearly identified as the unit cell. The dispersion tensor is found using the procedures illustrated in “Appendix B” as:

* DM*=

⎡

⎣ 11*.529e − 4.770e − 5* 11*.770e − 5 − 2.762e − 8.529e − 4 − 1.499e − 8*
*− 2.762e − 8 − 1.499e − 8 9.953e − 5*

⎤

⎦ MPa · ms2

(27)

*The averaged horizontal displacement u(x), i.e. the *
volu-metric average of horizontal displacement within a constant
*distance ls*, along the bar for two time instants is plotted

in Fig. 12*. In this study, ls* is equal to 1/500 of the total

length of the bar. According to the reference DNS solution, the input sinusoidal wave does not maintain its profile dur-ing the propagation and it breaks into several pulses with obvious magnitude decay. The profile also shows signifi-cant oscillations caused by reflections at material interfaces. The magnitude decay of the DNS model exhibits a more gradual process than the 1D wave propagation problem con-sidered in Sect.3.1. This is due to the two-dimensional nature of the microstructure. The coarse dispersive model captures the magnitude of the wave well although it predicts a more smooth wave profile. The computational time per time step for the dispersive multiscale model is around 0.04 seconds while for the DNS model around 2.5 seconds is needed on the same system (a PC with a 16 GB of memory and 3.5 GHz Intel Xeon CPU).

**4 RVE existence study**

In the previous section, the accuracy of the introduced dis-persive model has been validated for periodic composite structures in which an RVE can be clearly defined as the building unit cell. However, for engineering materials such as fiber reinforced composites, the assumption of a peri-odic microstructure is not representative. Spatial variations in the fiber distribution can affect the material response. The existence of an RVE for this multiscale approach needs to be assured before the dispersive multiscale model can be applied to simulate realistic composites with ran-dom microstructure. The definition of an RVE prescribes that the size should be sufficiently large such that fur-ther increase of the size does not lead to change in the

0 10 20 30 40 50 -0.01 -0.005 0 0.005 0.01 0.015 0.02 0.025 0.03 Fine heterogeneous (DNS) Fine homogenized Coarse non-dispersive Coarse dispersive (proposed)

0 10 20 30 40 50
-0.01
-0.005
0
0.005
0.01
0.015
0.02
0.025
0.03
)
m
m
(
e
t
a
n
i
d
r
o
o
-x
)
m
m
(
e
t
a
n
i
d
r
o
o
c
-x
Displacement
(mm)
Displacement
(mm)
**(a)** *t = 0.014 ms* **(b)** *t = 0.04 ms*

**Fig. 12 plots of displacement field at different time**

**(a)** **(b)** **(c)**

**Fig. 13 Processes for generation of numerical samples with periodic**

**boundary condition. a Initial configuration of a particle system (red**
arrows show a typical initial velocity field of particles and black arrows
**shows the diminishing motion); b intermediate configuration (dashed**

box shows the undiminished reference body, red particles with arrows
denoting the moving direction demonstrate the effect of periodic
**bound-ary condition); c final configuration: a numerical sample of composite**
microstructure. (Color figure online)

homogenized properties (or effective response). Therefore, the homogenized quantities, i.e. the dispersion tensor and the stiffness tensor, of random microstructures with dif-ferent sizes are calculated in this study. It is noted that with reference to undirectional fiber-reinforced composites circular inclusions are considered here while non-circular inclusions, for instance, ellipses with different aspect ratio, can be considered for other materials, following Li et al. [40]. In this section, the numerical tool used to gener-ate random microstructures is firstly described, followed by a study of the spatial distribution features of gener-ated numerical samples. Finally, convergence of the dis-persion tensor and stiffness tensor for realistic composite microstructure with respect to micromodel dimensions are presented.

**4.1 Generation of random microstructure with DEM**

Following van der Meer [41], a Discrete Element Method (DEM) solver called HADES, developed by Stroeven [42], is used to generate numerical samples of random microstruc-tures. DEM allows for generation of high packing density of granular samples, as the final configuration is a result of stochastic initial conditions and particle-to-particle collisions under external environment force and boundary conditions.

The process for generating a two-dimensional numerical
*sample with desired packing density Vi* is described as

fol-lows (see Fig. 13): A large box-shaped reference body is
**created initially, which contains a predefined number of N****i**

*circular particles with either a given constant diameter Di*or

posi-tions of the particles are random perturbaposi-tions of horizontally
and vertically aligned locations. The initial velocity of any
particle is prescribed to be the same in the horizontal and
ver-tical direction but with a randomly assigned magnitude and
sign for each particle. The reference body is gradually
dimin-ishing with the same velocity in the horizontal and vertical
direction (see Fig.13a). Periodic boundary conditions are
applied to the reference body to avoid any wall effect [17].
This means that during the simulation whenever a moving
particle is crossing the edge (or corner) of the diminishing
reference body, it reappears in the corresponding edge (or
corner) during the DEM simulation (see Fig.13b). The
col-lision between particles are treated with the Hertz contact
law [42]. The inter-particle contact can introduce energy
dis-sipation characterized by contact damping. In the case that
damping coefficients are non-zero, continuous energy loss
due to contact results in a clustering effect on the resulting
particle system. It will be demonstrated in Sect.4.2that this
phenomenon can be clearly demonstrated with the spatial
dis-tribution pattern of the particle system. A minimum contact
*distance parameter d*minis enforced so that any two particles

can not be closer than this value, following the same hard-core model concept as in [43–46]. It can be expected that decreasing the size of the reference body has the effect of increasing the volume fraction of particles. The simulation stops when the reference body has decreased such that the desired packing density, i.e. volume fraction, is reached (see Fig.13c). After this, a mesh is generated with GMSH [47] for the inclusions and the matrix.

**4.2 Spatial point distribution analysis**

For the random microstructure of composites reinforced
with long fibers, the inclusions can be considered as
dis-crete circular objects dispersed into a continuum matrix in
a two-dimensional domain. The spatial positioning of these
inclusions is stochastic for realistic composites due to the
manufacturing processes and conditions. By treating the
cen-ter of each inclusion as one point, statistical spatial point
pattern analysis can be applied to characterize the
microstruc-ture. As it is commented in Bailey and Gatrell [48], the basic
interest in analysing the spatial point process is in whether the
observed events exhibit any systematic pattern, as opposed
to being distributed randomly in space. Possibilities for these
patterns are classified as first order or second order effects.
First order effects relate to variation in the mean value of the
process in space representing a global trend in the
distribu-tion of inclusions. Second order effects result from the spatial
dependence in the process, representing a local effect. This
can be described by the probability density function of the
*nearest neighbour distances and Ripley’s K function [*48].

In this study, numerical samples of composite microstruc-tures generated by HADES are first evaluated for their

**(a)** **(b)**

**Fig. 14 A representative sample of a batch A and b batch B**

spatial distribution pattern. By introducing the contact damp-ing within the DEM solver, the inter-particle (inclusion) distances become smaller, representing local effects. To demonstrate the influence of contact damping, two batches of numerical samples are considered, one with nonzero contact damping (batch A) and the other with zero contact damp-ing (batch B). The probability density function of the nearest neighbour distances and Ripley’s K function are evaluated for these two batches of samples.

**4.2.1 Nearest neighbour distances**

The nearest neighbour distance (NND) measures the shortest
*inter-inclusion interaction. The N th (N* *= 1, 2, . . .) nearest*
neighbour distance is the distance between a randomly
*cho-sen inclusion and its N th closest neighbour in the studied*
domain [48]. It is assumed that the studied numerical sample
is in some sense representative of any region from a
real-istic composite microstructures. Therefore, it is needed to
determine at which size the NND distribution function has
converged. Eight different sizes are considered, by varying
*the number of inclusions per sample Ni* with values among

*[5 × 5, 10 × 10, 15 × 15, 20 × 20, 25 × 25, 30 × 30, 35 ×*
35*, 40 × 40]. By increasing the number of inclusions while*
keeping the volume fraction unchanged, the total volume
of the micromodel is also changed. For a given size, 100
random numerical samples are generated to ensure the
repre-sentativeness of possible spatial distributions. Representative
numerical samples of batch A and B are shown in Fig.14.
*The diameter of the inclusions Di*is kept as a fixed value of

5 *µm and their volume fraction Vi* is 60%. The minimum

*contact distance d*minis set to be 0.18µm.

In Fig.15a, the probability density of the 1st NND at
dif-ferent distances corresponding to difdif-ferent sample sizes for
batch A is shown. The value of the probability density at a
*distance h represents the “chance” of the 1st NND for an*
*inclusion to be h. A detailed view of the probability density*
of the 1st NND at two typical distances for different sample
sizes is plotted in Fig.15b. It is noted that in order to
elimi-nate the influence of the sample boundary on the probability

**Fig. 15 a The 1st NND for**

**different sample sizes; b 1st**
NND at two distances for
different sample sizes

5 5.2 5.4 5.6 5.8 6
0
2
4
6
8
10
12
*Ni*= 102
202
352
*Distance h (*μm)
Probability
density
(
μ*m*
−1
)
**(a)**
52_{10}2_{15}2 _{20}2 _{25}2 _{30}2 _{35}2 _{40}2
0
2
4
6
8
10
12
*h = 5*.24μm
5.30μm
*Number of inclusions Ni*
Probability
density
(
μ*m*
−
1)
**(b)**
5 5.2 5.4 5.6 5.8 6 6.2
0
2
4
6
8
10
12
Batch A (1st NND)
Batch B (1st NND)
Batch A (2nd NND)
Batch B (2nd NND)
*Distance h (*μm)
Probability
density
(
*m*
−1
)
μ

**Fig. 16 The probability density function of the 1st and 2nd NND for**

sample batch A and sample batch B (35× 35 inclusions)

density function of the 1st NND for a given numerical sam-ple (e.g. Fig.13c), a toroidal correction is applied. It assumes that the top and left of the sample domain is connected to the bottom and right, respectively, as if the sample domain is a torus [49,50]. It can be found from Fig.15that as the size of sample increases, the mean value of the 1st NND den-sity function gradually converges and the standard deviation decreases. When the sample has 35× 35 inclusions, the 1st NND function represents a size-independent function for this batch of samples. The same holds for the numerical samples of batch B. With this converged size, the probability density function of the 1st and 2nd NND for batch A and batch B are evaluated, with the mean value and standard deviation shown in Fig.16. It can be found that the largest probability of 1st NND occurs around 5.21µm for both batch A and batch B, however, batch A has a larger peak value than batch B. The 2nd NND shows the largest probability around 5.24µm for batch A while the largest probability for batch B occurs at around 5.38µm. Again, the peak value of batch A is larger than batch B. These observations show that the spatial dis-tribution of inclusions of batch A is more clustered than that of batch B, which is a result of the contact damping included for batch A.

**4.2.2 Ripley’s K function**

The nearest neighbour distance considers the point pattern on
the smallest scale. Information on larger scales is considered
*by Ripley’s K function [*48*]. The K function is the ratio*
between the expected number of inclusions within a circle
*of radius h of an arbitrary inclusion and the mean number*
*of inclusions per unit area. A direct estimate of K(h) from a*
numerical sample is given by [48]

*K(h) =* *A*
*N _{i}*2

*i*

*j=i*

*Ih(di j*

*≤ h)*

*wi j*(28)

*in which A is the area of the sample, Ni*is the total number of

*inclusions, di jis the distance between inclusion i and j , Ih(x)*

is an indicator function which has a value of 1 if the
*condi-tion x is true otherwise 0, andwi j*is a weighting function for

edge correction following Zangenberg and Brøndsted [50].
A homogeneous point process with no spatial dependence is
*the Poisson process with K* *= πh*2[48]. The mean value and
*standard deviation of the K function for batch A and B are*
plotted in Fig.17along with the Poisson solution. The
stan-dard deviations for the two batches are both very small. The

0 20 40 60
0
0.5
1
1.5
2·10
4
Batch A
Batch B
Poisson
*Distance h (*μm)
*K*
(
μ*m*
2)

52_{10}2_{15}2 _{20}2 _{25}2 _{30}2 _{35}2 _{40}2
0
1
2
·10−8
*Number of inclusions Ni*
*D*
*M* *ijk*
*l*
(MP
a·ms
2)
52_{10}2_{15}2_{20}2 _{25}2 _{30}2 _{35}2 _{40}2
0
1
2
·10−8
*Number of inclusions Ni*
*DM*
1111
*DM*
2222
*DM*
1212
*DM*
1122
*DM*
2212
*DM*
1112
**(a)** **(b)**

**Fig. 18 The dispersion tensor for sample a batch A and b batch B**

*mean value of the K functions for the two batches are very*
close to each other and both approach the Poisson distribution
for larger length scales. It is concluded that the first and
sec-ond NND provides a good indicator to distinguish between
different fiber distributions, while Ripley’s K function is less
informative.

**4.3 Convergence of dispersion tensor**

The influence of micromodel size on the dispersion tensor for
the two batches is investigated to examine the convergence
of the dispersion tensor. With the methodology mentioned
in Sect.2, the dispersion tensor can be solved using finite
element models. The material properties for inclusions are
*prescribed as the Young’s modulus Ei* = 74 GPa, Poisson’s

ratio*μi* *= 0.2, density ρi* = 2500 kg/m3and the matrix

*prop-erties are Young’s modulus Em* *= 3.76 GPa, Poisson’s ratio*

*μm* *= 0.3, density ρm* = 1200 kg/m3. There are six

indepen-dent components for the dispersion tensor due to symmetry.
Fig.18shows the mean value and standard deviation of the
individual components of the dispersion tensor for the
numer-ical samples of batch A and batch B. Again, 100 realizations
of the fiber distribution are solved for each batch and each
*Ni*.

There are several similar observations for the two batches.
*The mean and standard deviation of DM*_{1111}*and D*_{2222}*M* are very
close to each other, which means that no directional bias is
created with either the numerical samples or the dispersive
multiscale formulation. The mean values of the cross terms
*of DM*1112*and D*

*M*

2212are calculated to be very close to zero, as

expected for a transversely isotropic material. However,
cer-tain different findings can be made for the two batches. It is
seen that the mean value of the six independent components
of the dispersion tensor for batch A is gradually approaching a
*constant value after Ni*becomes larger than 202with

decreas-ing standard deviations. For batch B, the mean value of the
dispersion tensor components shows the trend of converging
*to a constant value after Ni*becomes larger than 302with the

standard deviations tend to decrease as well. The converged values of the dispersion tensor for these two batches seem to be different, which can be possibly due to different spatial distribution patterns. The dispersion tensor converges with a very large size for both these two batches, although for batch A the convergence rate is slightly faster.

**4.4 Convergence of stiffness tensor**

The influence of the numerical micromodel size on the stiffness tensor for the two batches is investigated to also examine convergence of the homogenized stiffness tensor. The stiffness matrix is obtained by using the numerical scheme explained in “Appendix A”. Plane-strain conditions are assumed herein. The calculated mean and standard devia-tion of the stiffness tensor is shown in Fig.19. It can be found that for both these two batches, the standard deviation values for the stiffness tensor are small compared with the mean val-ues. The mean values already converge for relatively small micromodel size. The calculated mean values of the stiffness tensor for batch A and batch B in matrix notation are:

* SM(A)*=
⎡
⎣ 155485302

*.1.2*155735302

*.1.9*

*−0.949295−3.99049*

*−3.99049 −0.949295*5125

*.54*⎤

*⎦ ,*

*= ⎡ ⎣ 152215184*

**S**M(B)*.62 15214.1 2.89584.1 5184.62 −4.87758*

*−4.87758 2.89584 5015.75*⎤ ⎦ (29)

* To verify the results, the isotropy of SM* is checked. It is
known that for isotropic material under plane strain
condi-tion, the stiffness matrix is

52_{10}2_{15}2_{20}2 _{25}2 _{30}2 _{35}2 _{40}2
0
0.5
1
1.5
·104
*Number of inclusions Ni*
*S*
*M* *ijk*
*l*
(MP
a)
*SM*
1111
**(a)**
52_{10}2_{15}2 _{20}2 _{25}2 _{30}2 _{35}2 _{40}2
0
0.5
1
1.5
·104
*Number of inclusions Ni*
*S*
*M* *ijk*
*l*
(MP
a)
*SM*
1111
*SM*
2222
*SM*
1212
*SM*
1122
*SM*
2212
*SM*
1112
*SM*
1111
**(b)**

**Fig. 19 Stiffness tensor for a batch A and b batch B. Enclosed subplots show the zoomed-in view of stiffness component S**_{1111}*M*

* SM* =
⎡
⎢
⎢
⎣

*S*

_{1111}

*M*

*S*

_{1122}

*M*

*S*

_{1112}

*M*

*S*

_{2211}

*M*

*S*

_{2222}

*M*

*S*

_{2212}

*M*

*S*

_{1211}

*M*

*S*

_{1222}

*M*

*S*

_{1212}

*M*⎤ ⎥ ⎥ ⎦ =

*E*

*(1 + ν)(1 − 2ν)*⎡ ⎣1

*− ν*1

_{ν}*− νν*00 0 0 1

*−2ν*

_{2}⎤ ⎦ (30)

*where E is the Young’s modulus and* *ν is the *
Pois-son’s ratio. Therefore, an isotropic law should satisfy that
*2S*_{1212}*M* */(S*_{1111}*M* *− S*_{1122}*M* *) is equal to one. An error *
measure-ment*S*is introduced as
*S*=
*2S*_{1212}*M*
*(SM*
1111*− S*
*M*
1122*)*
− 1_{}× 100% (31)
According to Eqs. (29) and (31), the errors for batch A and
batch B are calculated to be 0.0486% and 0.0496%,
respec-tively. This shows that the calculated stiffness is very close
to theoretical values. As it is seen in Eq. (29), the difference
between any component of the calculated stiffness tensor for
these two batches is less than 2%, which means that the
stiff-ness tensor is not sensitive to the considered differences in
spatial distribution of the microstructure.

**5 Experimental calibration**

It is demonstrated in Sect. 4 that the convergence per-formance of the dispersion tensor depends on the spatial distribution pattern of the inclusions. Therefore, realistic microstructures should be studied to evaluate the appropriate-ness of this method to be applied in real composite structures. With image-analysis techniques, spatial distribution patterns can be extracted from snapshots of real composites (see e.g.

Czabaj et al. [51]). Computational approaches can thereafter be used to generate random numerical samples according to the experimentally determined spatial patterns.

In this study, numerical samples are generated with the
DEM solver HADES for the microstructure of a CFRP
com-posite, HTA/6376, with a fiber volume fraction of 59.2%
[52,53]. First, the DEM settings are calibrated to match
experimentally observed NNDs. Then, the RVE existence
study from the previous section is repeated with these
set-tings. For the calibration the number of fibers is fixed at
1296 (= 362_{) in line with the experimental observations}

on 1300 fibers. The adopted RVE size is large enough to
consider the spatial distribution in the numerical samples as
representative based on the observation in Fig. 15. A fiber
diameter distribution function is predefined according to the
experimentally determined size distribution (see Fig. 20).
The contact parameters, i.e. damping and minimum distance
*d*min of the DEM simulation are tuned such that the

spa-tial distribution pattern of generated numerical samples can match the experimentally-determined patterns. Herein, 100 numerical samples are generated with the DEM solver. The mean value and standard deviation of the actual fiber

diam-5.5 6 6.5 7 7.5 0 0.05 0.1 0.15 Diameter (μm) Frequenc y Experiment [52] This study

5 5.5 6 6.5 7 7.5 8 8.5 9
0
0.5
1
1.5
2
2.5
3
*Distance h (*μm)
Probability
density
(µ
*m*
−
1)
Yang et al. [43]
Ismail et al. [54]
This study
Experiment [52]

**Fig. 21 The probability density function of 1st NND**

eter distributions used in the DEM simulations are shown in Fig.20along with the experimental quantification to ver-ify that the input distribution is recovered. The calculated mean and standard deviation of the probability density func-tion of the 1st NND for the calibrated numerical samples are demonstrated in Fig.21along with the experimental result and two reference solutions from other numerically gener-ated fiber distributions by Yang et al. [43] and Ismail et al. [54]. It is seen that the probability density function of the 1st NND for the generated numerical samples has a good match with the experimental measurements. A considerably better agreement is found for the current study than for the two reference solutions. The mean and standard deviation of the probability density function of the 2nd NND for the numerical samples and the reference solutions are shown in Fig.22. Again, the result for the generated numerical samples matches well with the experiment measurements. A higher agreement is found for this study than Yang et al. [43] while the solution from Ismail et al. [54] also shows a good match. It is therefore validated that the generated numerical samples

5 5.5 6 6.5 7 7.5 8 8.5 9 9.5 10
0
0.5
1
1.5
2
*Distance h (*μm)
Probability
density
(μ
*m*
−1
)
Yang et al. [43]
Ismail et al. [54]
This study
Experiment [52]

**Fig. 22 The probability density function of 2nd NND**

52102152202 252 302 352 402
0
1
2
3
·10−8
*Number of fibers Nf*
*D*
*M* *ijk*
*l*
(MP
a·
ms
2)
*DM*
1111
*DM*
2222
*DM*
1212
*DM*
1122
*DM*
2212
*DM*
1112

**Fig. 23 Convergence study of calibrated sample**

are sufficiently representative for the real microstructure of the CFRP composite, following the criterion proposed by Liu and Ghoshal [55].

A convergence study on the dispersion tensor is performed
next by increasing the size of samples with the same DEM
solver settings as the calibrated numerical samples. Again,
eight different sizes are considered, and for every size 100
random numerical samples are generated and solved for the
dispersion tensor with the FEM model. The influence of the
micromodel size on the six independent components of the
dispersion tensor is plotted in Fig.23. The standard
devia-tion of all six components shows a decreasing trend as the
*number of fibers Nf* is larger than 400 and the mean values

converge to representative values. This means that for this specific composite material the dispersion tensor components converge although convergence is still relatively slow when compared with the stiffness tensor components as shown in Fig. 19 or the elasto/plastic response of composites as reported in [41].

**6 Conclusion**

In this paper, a multiscale model is introduced to capture wave dispersion in composites. By using asymptotic homogeniza-tion, it is found that the dispersion effect can be characterized by a dispersion tensor, the magnitude of which is dependent on the material property contrast of inclusion/matrix and the size of the inclusion. The dispersive multiscale model is applied to simulate elastic wave propagation problems in a bar with one-dimensional and two-dimension microstruc-tures. Comparison with a DNS model shows that the disper-sive multiscale model has a significantly improved accuracy, compared with non-dispersive homogenized models. To test if an RVE can be defined for realistic composites with random microstructures, the dispersion tensor and stiffness tensor are

computed for random numerical samples at different sizes. It
is found that the convergence performance of the dispersion
tensor is considerably slower than that of the stiffness tensor
and that the convergence depends on the spatial distribution
pattern. Finally, a batch of calibrated numerical samples of
CFRP composites is tested for the convergence of the
disper-sion tensor. It is argued that careful definition of
microstruc-ture geometries is required to achieve representativeness.
**Acknowledgements Financial support from the China Scholarship**

Council is gratefully acknowledged by YL.

**Open Access This article is distributed under the terms of the Creative**

Commons Attribution 4.0 International License (http://creativecomm ons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.

**Appendix A**

The solution of Eq. (18) follows a standard FEM formulation
with the precomputation of the dispersion tensor via the
pro-cedures in Sect.2.1.3. The stiffness matrix is needed for the
calculation of the macro-scale stress*σ _{i j}(0)*. This is obtained by
a standard computational-homogenization scheme following
Karamnejad and Sluys [32]. Periodicity is assumed for the
boundary edges and a prescribed displacement is applied to
three controlling nodes (see Fig.24) according to

* ui* = ˜

*(32)*

**H**i**ε**M, i = 1, 2, 4where* εM*is the macro-scale strain and

˜
* Hi* =
⎡
⎢
⎢
⎣

*y*

_{1}

*i*0 0

*y*

_{2}

*i*

*y*

_{2}

*i*2

*yi*

_{1}2 ⎤ ⎥ ⎥ ⎦ (33) 1 2 4 3 Γ

*B*Γ

*T*Γ

*L*Γ

*R*

**Fig. 24 Periodicity of RVE. Two periodicity pairs of edges:***L* and

*R*;*T*and*B*

After solving the incremental form of system equation
* Kδu = δ f , the stiffness matrix SM* is obtained by

* SM* = ˜

*1*

**H***˜2*

**H***˜4*

**H***−1*

**K**pp**− K**p f**(K**f f)*⎡ ⎣*

**K**f p*˜˜12 ˜*

**H****H***4 ⎤ ⎦ (34)*

**H***in which subscript p denotes the degrees of freedom of the*

*three controlling nodes and subscript f represents the other*free nodes.

**Appendix B**

To solve Eq. (24), the influence function *hmn _{k}*

*(mn= 11, 22, 12) is treated as nodal variable. In matrix*

**nota-tion, standard FEM formulation with h**mn_{:= (h}mn1 *, h*

*mn*

2 *)T* =

* N hmn* and

**ω = Nω are introduced where N is the shape***,*

**function matrix and h**mn*the acceleration influence function and test function, respec-tively. Equation (24) is further simplified by using the FEM formulation as*

**ω contain the nodal values of**

**(Lω)**T**mn**_{σ}**T**_{+ (Lω)}

**F**mn*d*

**= ω**T

**B**T**σ**mn**+ B**T**F**mn*d = 0*(35) where

*⎡ ⎢ ⎣*

**Lω =***∂*

*∂ y1*0 0

_{∂ y2}∂*∂*

*∂ y2*

*∂ y1∂*⎤ ⎥ ⎦

*ω*1

*ω*2 = ⎡ ⎣

*ω*2

_{ω}(1,1)_{(2,2)}*ω*⎤ ⎦

_{(1,2)}

**σ**mn_{=}⎡ ⎣

*σ*

*mn*11

*σmn*22

*σmn*12 ⎤ ⎦ = ⎡ ⎣

*SS*11112211

*SS*11222222

*SS*11122212

*S*1211

*S*1222

*S*1212 ⎤ ⎦ ⎡ ⎢ ⎣

*hmn*

_{(1,1)}*hmn*

_{(2,2)}*2hmn*⎤ ⎥ ⎦

_{(1,2)}*= ⎡ ⎣*

**F**mn*F*

*mn*11

*F*

_{22}

*mn*

*F*

_{12}

*mn*⎤

*⎦ = ρ(*⎡ ⎣

_{ρ}_{(0)}**y**)*SS11mn22mn*

*S12mn*⎤ ⎦

**in which the matrix B****= LN.**The constraint equation Eq. (12) is rewritten as
*hmnk* * _{}*=
!

*"*

**N h**mn

**= N****h***mn*

*= 0 (36)*

**= ch**mn*. Equation (36) can then be treated as a constraint for the linear system of equa-tions given by Eq. (35*

**in which the cofficient matrix c****= N**_{}

**). The y−periodicity condition of h**mn_{k}can be enforced directly by periodicity constraints on corre-sponding edges of the RVE (see Fig.24).